# Dopants in Lanthanum Manganite: Insights from First-Principles · PDF fileDopants in Lanthanum...

Embed Size (px)

### Transcript of Dopants in Lanthanum Manganite: Insights from First-Principles · PDF fileDopants in Lanthanum...

Dopants in Lanthanum Manganite: Insights from First-PrinciplesChemical Space ExplorationSridevi Krishnan,*,, Vinit Sharma,,, Prabhakar Singh,, and Rampi Ramprasad*,,

Materials Science and Engineering, University of Connecticut, Storrs, Connecticut 06269, United StatesInstitute of Materials Science, University of Connecticut, Storrs, Connecticut 06269, United StatesCenter for Clean Energy Engineering, University of Connecticut, Storrs, Connecticut 06269, United States

*S Supporting Information

ABSTRACT: The dopant chemical space in LaMnO3 (LMO) is systematically explored using first-principles computations. Westudy a range of cationic dopants including alkali, alkaline earth metals, 3d, 4d, and 5d transition metal elements without and withan adjacent O vacancy. A linear programming approach is employed to access the energetically favorable decomposition pathwayand the corresponding decomposition energy of doped LaMnO3. The decomposition energy is then used to classify the dopantsfor stability, site preference and tendency of O vacancy formation. We find that La site doping is more favored compared to Mnsite doping. We also identify dopants previously not considered, such as K, Rb, Cs, and In, which lead to stable doped LMO andare also excellent O vacancy formers. Employing data mining techniques, we identify the dopant features that are critical to thestability of a doped oxide.

INTRODUCTIONOxide perovskites are an attractive class of materials with abroad array of technological applications,1,2 owing to theirexceptional physical and chemical properties. The remarkableability of the perovskite structure with the generic formulaABO3 to host a variety of A and B site cationic elements leadsto different materials with a host of interesting properties. Inaddition, doping in either of the cationic sites opens up avenuesfor further tailoring the material properties. Doped lanthanumManganite (LaMnO3 or LMO) is one such oxide perovskitewith an array of applications35 including in solid oxide fuelcells,6,7 giant magneto resistance devices,8 and catalyticcombustion.9 Although a few dopants in LMO have beenexplored,1016 a comprehensive study of the many possibledopants at a consistent level of theory is unavailable at thistime. Such a study will provide very useful insights pertaining tothe stability of a dopant in LMO or similar oxide.In recent years, the community has resorted to large scale

chemical space searches (via high-throughput computing) inwhich several possible candidates are initially considered in anunbiased and uniform manner.1729 Such a strategy isparticularly useful either when chemical intuition concerning

the relevant cases are unavailable (thereby preventing furthersignificant progress), or when predictive models based onquantitative trends and correlations across a chemical series isdesired. Indeed, these strategies have led to several successfuldiscoveries of new materials.3037

Here, we employ a systematic search of the dopant chemicalspace to identify stable and desirable dopants in LMO. To aidthis search, we explore cationic dopants ranging from the alkaliand alkaline earth metals, 3d, 4d, and 5d series transition metalsthrough group VA of the periodic table (KAs, RbSb, andCsBi) amounting to a total of 44 dopants. In order to probethe role of the dopant on O chemistry, all doped cases wereconsidered without and with an O vacancy adjacent to thedopant atom.A linear programming approach was used to determine the

energetically most favorable decomposition pathway (orproducts) if any, for each case, and the correspondingdecomposition energy. The dopants were then assessed based

Received: May 4, 2016Revised: July 18, 2016Published: July 26, 2016

Article

pubs.acs.org/JPCC

2016 American Chemical Society 22126 DOI: 10.1021/acs.jpcc.6b04524J. Phys. Chem. C 2016, 120, 2212622133

pubs.acs.org/JPCChttp://dx.doi.org/10.1021/acs.jpcc.6b04524

on the resistance of the doped oxide to decomposition, thetendency of O vacancy formation and the site preference basedon the decomposition energy.Our strategy correctly recovers dopants already known to be

efficacious for enhancing O vacancy formation in LMO.Additionally, we identify new dopants, including K, Rb, Csand In, which are expected to lead to stable doped LMO thatare simultaneously superior O vacancy formers. This trend isvisually captured in Figure 1, which displays the stability ofdoped LMO with the dopant in the A or B site and without orwith an adjacent O vacancy (green shades indicate cases andsituations with high stability). Data mining methods38 wereemployed to identify trends and correlations between thedopant properties and the stability of the compounds. It ishoped that this work will spur future experimental studies ofthese doped oxides.

METHODSModels. The room temperature structure of LMO is

orthorhombic;39 however, applications involving high temper-ature operations like SOFC, the structure becomes cubic.Therefore, we chose the cubic perovskite structure for all ourcalculations. We then substitutionally doped the cations KAs,RbSb, and CsBi at the La or Mn sites in a 2 2 2supercell, resulting in a dopant concentration of 12.5%. Inaddition, a neutral O vacancy in the vicinity of each dopant wasconsidered. Altogether, four different sets of calculations withdopants (D) in the La (La1aDaMnO3) and Mn (LaM-n1aDaO3) sites without ( = 0) and with ( = 0.125) an Ovacancy were performed. For consistency, all of the compoundswere initialized in a ferromagnetic (FM) state and allowed torelax to their ground state.Computational Details. Spin polarized calculations were

performed using density functional theory as implemented inthe VASP40,41 code. The electron exchange-correlationinteraction was treated using the generalized gradientapproximation (GGA) with PerdewBurkeErnzerhof(PBE)42 functional. The projector augmented wave (PAW)potentials43 were used to describe the core states. Allcalculations were performed with a cutoff energy of 520 eV

and a 4 4 4 MonkhorstPack k-point grid was used tosample the brillouin zone. The atomic positions were relaxed inthe cubic supercell until the force on each atom fell below athreshold of 0.02 eV/.

Stability. Conventionally, the thermodynamic stability of adoped compound is estimated from the calculated formationenergy. The formation energy can be defined in multiple waysdepending on the reference chosen for elemental chemicalpotentials.However, what is more relevant to stability is the tendency of

a compound, once formed, to resist decomposition. Thedecomposition energy of a compound such as doped LMO isfar more difficult to compute than an appropriately definedformation energy, as there can be a plethora of decompositionproducts, including some combination of the relevant metallicelements/alloys, binary oxides and ternary oxides.In order to find the most expected decomposition pathway,

all the possible combinations of the decomposition reactionsshould be studied and their corresponding energies compared.Alternatively, a constrained optimization can find the mostthermodynamically favored set of products subject tostoichiometry preserving constraints (as described below).The linear programming (LP) method4448 offers an efficient

approach to find the most expected set and amounts ofproducts for the doped compounds. This involves listing thepossible product compounds (the product pool), which inour case included the elemental metals, their binary oxides,LMO and oxygen molecule. The coefficients ci correspondingto each of these product compounds represent the amount ofeach product compound contained in the final set of products.The decomposition energy of a doped LMO with dopant D,EdD, is then defined as

=

+ +

+ +

+

+ +

E E min

c E c E c E

c E c E

c E

c E c E

dD

LMOD

c

La s Mn s D s

La O s Mn O s

D O s

LaMnO O

1 ( ) 2 ( ) 3 ( )

4 ( ) 5 ( )

6 ( )

7 8

i y x

2 3 2 3

3 2 (1)

Figure 1. Dopants from the periodic table considered in this study. The decomposition energy (EdD) of the compound with a substitutional dopant in

the La and Mn site both without and with an adjacent O vacancy in the vicinity of the dopants is represented by the left, bottom, top and righttriangles, respectively. The decomposition energy is color coded and the color bars shows the scale for the decomposition energy. The dopedcompound is considered stable against decomposition when Ed

D < 0 eV. The gray line connecting the dots represents the string for Mendeleevnumber ordering.

The Journal of Physical Chemistry C Article

DOI: 10.1021/acs.jpcc.6b04524J. Phys. Chem. C 2016, 120, 2212622133

22127

http://dx.doi.org/10.1021/acs.jpcc.6b04524

where ELMOD is the DFT energy of the doped compounds (with

the dopant at the La or the Mn site, and with or without anadjacent O vacancy) and all the Es in the second term are DFTenergies of all possible elemental, binary and ternary oxidesconsidered as products.The ci coefficients that minimize the second term of eq 1 are

determined subject to the following stoichiometry preservationconstraints:

+ + =

+ + =+ =

+ + + + =

c c c a

c c c

c yc a

c c xc c c

2 1

2 1

3 3 3 2 3

1 4 7

2 5 7

3 6

4 5 6 7 8 (2)

c 0i (3)

To understand the above constraints, let us consider anexample. The stoichiometry of La in La1aDaMnO3 is 1 a;thus, the sum of all cis of compounds involving La (namely c1,c4, and c7) should be equal to 1 a, leading to the first equalityof eq 2. The minimization of the second term in the right-handside of eq 1 subject to the constraints in eq 2 and 3 will le